#------------------------------------------------------------------------------
#$Date: 2021-06-15 10:12:38 +0200 (mar 15 de jun de 2021) $
#$Revision: 266469 $
#$URL: svn://www.crystallography.net/cod/cif/1/56/34/1563489.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1563489
loop_
_publ_author_name
'Souilah, M.'
'Lafond, A.'
'Guillot-Deudon, C.'
'Harel, S.'
'Evain, M.'
_publ_section_title
;
 Structural investigation of the Cu2Se--In2Se3--Ga2Se3 phase diagram,
 X-ray photoemission and optical properties of the
 Cu1−z(In0.5Ga0.5)1+z/3Se2 compounds
;
_journal_issue                   10
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              2274
_journal_page_last               2280
_journal_paper_doi               10.1016/j.jssc.2010.08.014
_journal_volume                  183
_journal_year                    2010
_chemical_formula_moiety         'Cu0.4 Ga0.6 In0.6 Se2'
_chemical_formula_sum            'Cu0.4 Ga0.6 In0.6 Se2'
_chemical_formula_weight         294.1
_space_group_IT_number           121
_space_group_name_Hall           'I -4 2'
_space_group_name_H-M_alt        'I -4 2 m'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  'I -4 2'
_symmetry_space_group_name_H-M   'I -4 2 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.63351(13)
_cell_length_b                   5.63351(13)
_cell_length_c                   11.2411(3)
_cell_measurement_reflns_used    30727
_cell_measurement_temperature    293
_cell_measurement_theta_max      39.97
_cell_measurement_theta_min      6.53
_cell_volume                     356.752(15)
_computing_cell_refinement       unknown
_computing_data_collection       unknown
_computing_data_reduction        unknown
_computing_molecular_graphics    unknown
_computing_structure_solution    unknown
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.98
_diffrn_measurement_device       'four-cycle diffractometer'
_diffrn_measurement_device_type  'Nonius CCD'
_diffrn_measurement_method       omega
_diffrn_radiation_monochromator  unknown
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0666
_diffrn_reflns_av_sigmaI/netI    0.012
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            30727
_diffrn_reflns_theta_full        39.97
_diffrn_reflns_theta_max         39.97
_diffrn_reflns_theta_min         6.53
_exptl_absorpt_coefficient_mu    30.78
_exptl_absorpt_correction_T_max  0.3277
_exptl_absorpt_correction_T_min  0.1087
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
'Jana2006  (Petricek, Dusek & Palatinus, 2000)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    5.4732
_exptl_crystal_description       block
_exptl_crystal_F_000             510
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.06
_refine_diff_density_max         1.56
_refine_diff_density_min         -1.96
_refine_ls_extinction_coef       680(140)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    1.85
_refine_ls_goodness_of_fit_ref   1.90
_refine_ls_number_constraints    3
_refine_ls_number_parameters     25
_refine_ls_number_reflns         1943
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0778
_refine_ls_R_factor_gt           0.0505
_refine_ls_shift/su_max          0.0065
_refine_ls_shift/su_mean         0.0010
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(σ²(I)+0.0016I²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.1283
_refine_ls_wR_factor_ref         0.1493
_reflns_number_gt                1517
_reflns_number_total             1943
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            JSSC-2010_183-2274.cif
_cod_data_source_block           9
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'Gaussian' was
changed to 'gaussian' in accordance with the built-in table derived
from the CIF Core dictionary named 'cif_core.dic' version 2.4.5 last
updated on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_cell_volume        356.7512
_cod_database_code               1563489
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 x,y,z
2 -x,-y,z
3 y,-x,-z
4 -y,x,-z
5 -x,y,-z
6 x,-y,-z
7 -y,-x,z
8 y,x,z
9 x+1/2,y+1/2,z+1/2
10 -x+1/2,-y+1/2,z+1/2
11 y+1/2,-x+1/2,-z+1/2
12 -y+1/2,x+1/2,-z+1/2
13 -x+1/2,y+1/2,-z+1/2
14 x+1/2,-y+1/2,-z+1/2
15 -y+1/2,-x+1/2,z+1/2
16 y+1/2,x+1/2,z+1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu_2a Cu 0 0 0 Uani 0.0181(5) 2 0.8 d . . .
In_4d In 0 0.5 0.25 Uani 0.0197(4) 4 0.1 d . . .
Ga_4d Ga 0 0.5 0.25 Uani 0.0197(4) 4 0.6 d . . .
In_2b In 0.5 0.5 0 Uani 0.0223(2) 2 1 d . . .
Se_8i Se 0.24058(12) 0.24058(12) 0.13033(7) Uani 0.0252(3) 8 1 d . . .
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cu 0.320 1.265 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
In -0.728 1.310 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Ga 0.231 1.608 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Se -0.093 2.226 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Se_8i Cu_2a Se_8i . . 2_555 105.21(3) yes
Se_8i Cu_2a Se_8i . . 3_555 111.64(2) yes
Se_8i Cu_2a Se_8i . . 4_555 111.64(2) yes
Se_8i Cu_2a Se_8i 2_555 . 3_555 111.64(2) yes
Se_8i Cu_2a Se_8i 2_555 . 4_555 111.64(2) yes
Se_8i Cu_2a Se_8i 3_555 . 4_555 105.21(3) yes
Se_8i In_4d Se_8i . . 2_565 111.97(3) yes
Se_8i In_4d Se_8i . . 11_455 108.24(2) yes
Se_8i In_4d Se_8i . . 12_555 108.24(2) yes
Se_8i In_4d Se_8i 2_565 . 11_455 108.24(2) yes
Se_8i In_4d Se_8i 2_565 . 12_555 108.24(2) yes
Se_8i In_4d Se_8i 11_455 . 12_555 111.97(3) yes
Se_8i Ga_4d Se_8i . . 2_565 111.97(3) yes
Se_8i Ga_4d Se_8i . . 11_455 108.24(2) yes
Se_8i Ga_4d Se_8i . . 12_555 108.24(2) yes
Se_8i Ga_4d Se_8i 2_565 . 11_455 108.24(2) yes
Se_8i Ga_4d Se_8i 2_565 . 12_555 108.24(2) yes
Se_8i Ga_4d Se_8i 11_455 . 12_555 111.97(3) yes
Se_8i In_2b Se_8i . . 2_665 109.34(2) yes
Se_8i In_2b Se_8i . . 3_565 109.54(2) yes
Se_8i In_2b Se_8i . . 4_655 109.54(2) yes
Se_8i In_2b Se_8i 2_665 . 3_565 109.54(2) yes
Se_8i In_2b Se_8i 2_665 . 4_655 109.54(2) yes
Se_8i In_2b Se_8i 3_565 . 4_655 109.34(2) yes
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Cu_2a Se_8i . . 2.4125(7) yes
Cu_2a Se_8i . 2_555 2.4125(7) yes
Cu_2a Se_8i . 3_555 2.4125(7) yes
Cu_2a Se_8i . 4_555 2.4125(7) yes
In_4d Se_8i . . 2.4046(7) yes
In_4d Se_8i . 2_565 2.4046(7) yes
In_4d Se_8i . 11_455 2.4046(7) yes
In_4d Se_8i . 12_555 2.4046(7) yes
Ga_4d Se_8i . . 2.4046(7) yes
Ga_4d Se_8i . 2_565 2.4046(7) yes
Ga_4d Se_8i . 11_455 2.4046(7) yes
Ga_4d Se_8i . 12_555 2.4046(7) yes
In_2b Se_8i . . 2.5334(7) yes
In_2b Se_8i . 2_665 2.5334(7) yes
In_2b Se_8i . 3_565 2.5334(7) yes
In_2b Se_8i . 4_655 2.5334(7) yes
